Growth kinetics of MPS-capped CdS quantum dots in self-assembled thin films
© Koç et al.; licensee Springer. 2012
Received: 18 July 2012
Accepted: 9 October 2012
Published: 5 November 2012
For this study, we prepared colloidal CdS quantum dots using 3-mercaptopropyltrimethoxysilane as capping agent. Colloidal CdS quantum dots were directly deposited on glass substrates by a spin-coating process. Coated substrates were heat-treated between 225°C and 325°C for various heat treatment time intervals to investigate the growth kinetics of the quantum dots. Results showed that sizes of the CdS quantum dots grew approximately from 2.9 to 4.6 nm, and the E1s 1s energy values shifted approximately from 3.3 to 2.7 eV. Results showed that the average size of quantum dots increase by thermal treatment due to Ostwald ripening. The thermal process used to grow the size of quantum dots was examined according to the Lifshitz-Slyozov-Wagner theory. The activation energy of CdS quantum dots in thin films was calculated at approximately 44 kJ/mol.
KeywordsCdS quantum dots 3-Mercaptopropyltrimethoxysilane Growth kinetics Ostwald ripening Thin films 81.07.Ta 81.16.Dn 65.80.-g
Unlike bulk materials, optical and electronic properties of nanoparticles depend on their crystal dimension due to quantum confinement effect. Therefore, many research have focused on the production of nanomaterials that have controllable size [1–11]. Several techniques have been used to control the growth process of nanoparticles. One of the most important technique is the growth of nanoparticles in glasses. Generally, high heat treatment temperatures over 550°C were needed to control the growth process of nanoparticles for this technique [1–3]. Nanoparticles can also grow by chemical reactions in liquid or thin film media. Low heat treatment temperature and very narrow size distributions of nanoparticles in liquid or in thin film media are the obvious advantages compared with the growth of nanoparticles in glasses [4–11].
CdS thin films and nanoparticles have been widely used in the area of optoelectronics. CdS nanoparticles and thin films can be produced by several methods [10–13]. One of these is the use of capping agents to produce colloidal CdS quantum dots. 3-Mercaptopropyltrimethoxysilane (MPS) contains a bifunctional group molecule; the silane on one side can bond to the glass surface or metal oxide films, and the thiol group on the other side can work as a capping agent [11, 12, 14]. Addition of MPS in the solvent will serve as a precursor for the growth of SiO2 to incorporate quantum dots in a silica matrix . SiO2 is an ideal shell material for CdS nanoparticles because SiO2 has a wide bandgap (9.1 eV) and an amorphous film structure .
Results show that the average size of quantum dots increases with the increasing heat treatment temperature and that small nanocrystals are dissolved with the increasing heat treatment temperature, and they are redeposited on the larger crystals due to Ostwald ripening. However, the effect of the capping agent thereby makes the growth process complex . The amount of capping agent will affect the interfacial diffusion and hence the solubility of the nanocrystals. This phenomenon is attributed to the results on capped CdS quantum dots which were previously reported by Zhang et al. . They said that ‘the growth of these QDs [quantum dots] was found to follow Ostwald ripening during the reflux process. When the amount of capping agent used exceeds some saturation value, an unprecedented dimerization of QDs is detected’. Fortunately, other effects can be neglected for Ostwald ripening if the appropriate amount of capping agent is used. Therefore, the amount of capping agent is selected in such a way that the bonding should neither be too strong nor too weak to allow for dynamic coupling in which the coordinating molecules attach and de-attach from growing nanoparticles .
In the present work, colloidal CdS quantum dots were directly deposited on glass substrates by spin-coating process. Therefore, self-assembled films made of CdS quantum dots in a SiO2 network were obtained using only one production step. The coated substrates were heat-treated between 225°C and 325°C for various time intervals to investigate the growth kinetics.
Production of quantum dots
CdS quantum dots were produced using the reaction of cadmium acetate (Cd(CH3COO)2·2H2O) with thioacetamide (CH3CSN2) at a molar ratio of one. Cadmium acetate and thioacetamide were first dissolved with methanol in separate beakers. The molar ratios of cadmium acetate/methanol and thioacetamide/methanol were equal to 0.02. MPS (HS(CH2)3Si(OCH3)3) was mixed with cadmium acetate at a molar ratio of MPS/Cd = 0.3 . This ratio was decided after analyzing the absorption spectrum of the nano CdS at several other ratios (0.1, 0.2, 0.5) and after considering previous works [11, 15, 19]. The solutions in two beakers were then mixed and stirred for 10 min at 60°C in nitrogen medium.
Production of thin films
MPS-capped CdS quantum dots were coated as thin film on a glass substrate (Corning 2947, Corning Incorporated, Tewksbury, MA, USA) by spin coating. The system was spun at a rate of 2,000 rev/min for 10 seconds. The substrate was heat-treated at 60°C for 10 min at each coating. The coated substrates were then heat-treated between 225°C and 325°C for various time intervals to investigate the growth kinetics. As explained in our previous work , during the formation of thin films, we suppose that quantum dots were attached to the glass surface by Si-O-Si bonds created by the OH group of the glass surface and the Si-O group of MPS.
High-resolution transmission electron microscopy (HRTEM) images and energy-dispersive X-ray spectroscopy (EDS) spectra of the MPS-capped CdS quantum dots in powder form were recorded using a JEOL 2100 (JEOL Ltd., Akishima, Tokyo, Japan) HRTEM microscope operated at 200 kV. X-ray photoelectron spectroscopy (XPS) spectra measurements of the thin films were carried out by SPECS PHOIBOS-150 Electron Analyzer (SPECS GmbH, Berlin, Germany) with a monochromatic X-ray source (Al-Kα) of photon energy 1,486.6 eV. Absorbance of the thin films was recorded with a UV-visible spectrometer (Agilent 8453, Agilent Technologies, Inc., Santa Clara, CA, USA).
Results and discussion
HRTEM and EDS
where E g is the bandgap energy of the bulk material (2.42 eV for CdS), r is the radius of the nanoparticle, m e * and m h * are the effective mass values of electrons and holes, respectively, (m e * = 0.19m0 and m h * = 0.8m0 for CdS), and ε is the dielectric constant (5.7 for CdS) . The average particle size of these films is calculated by inserting E1s 1s values into Equation 1. The results of the calculations showed that the average E1s 1s values decreased from 3.3 eV (for films dried at 60°C for 10 min) to 2.7 eV (for films heat-treated at 325°C for 60 min), and sizes of the CdS quantum dots increased from 2.9 to 4.6 nm. The results show that the redshift of E1s 1s values with increasing heat treatment temperature is due to the increasing nanocrystal size (quantum size effect).
The growth of nanocrystals can be described in terms of three stages: nucleation, normal growth stage, and Ostwald ripening. Size of nanocrystals is determined by the monomer concentration, capping ligand, and temperature at the nucleation and growth stages. At a fixed monomer concentration, Ostwald ripening dominates between nanoparticles. At this stage, the coarsening effects are characterized by diffusive mass transfer from smaller particles to larger ones, and the final size of nanocrystals is thus determined by temperature and time period of the Ostwald ripening . We are going to look at the growth process of the films at this stage.
where D is the diffusion coefficient, γ is the interfacial energy, V m is the molar volume, C∞ is the equilibrium concentration at a flat surface, ℜ is the gas constant, and T is the temperature.
where D0 is a coefficient independent of temperature, ℜ is the gas constant, and T is the heat treatment temperature. Q d is the (activation) energy of 1 mol of atom to make a diffusion movement.
In the present study, colloidal MPS-capped CdS quantum dots were self-assembled directly on a glass substrate using spin-coating method without introducing any matrix. The coated substrates were heat-treated to investigate the growth kinetics. Results showed that the average size of quantum dots changed from 2.9 to 4.6 nm when the heat treatment temperature and its duration time were increased. Compared to the growth of nanoparticles in glasses [2, 3], the present growing method has the advantage of lower activation energy and lower heat treatment temperature, but the presence of a capping agent may prevent the growth to larger values. The applied techniques work well for CdS nanocrystalline particles and enable one to prepare a series of samples with well-defined particle radii.
The authors would like to thank to Prof. Dr. Mustafa Ürgen for the XPS measurements. This work is supported by the Research Fund of Istanbul Technical University.
- Woggon U: Optical Properties of Semiconductor Quantum Dots. Berlin: Springer; 1997.
- Yükselici H, Persans PD, Hayes TM: Optical studies of the growth of Cd1−xZnxS nanocrystals in borosilicate glass. Phys Rev B 1995, 52: 11763–11772. 10.1103/PhysRevB.52.11763View Article
- Fuyu Y, Parker JM: Quantum size effects in heat treated, Cd(S, Se) doped glass. Mater Lett 1988, 6: 233–237. 10.1016/0167-577X(88)90028-6View Article
- Herron N, Wang Y, Eckert H: Synthesis and characterization of surface-capped, size-quantized CdS clusters: chemical control of cluster size. J Am Chem Soc 1990, 112: 1322–1326. 10.1021/ja00160a004View Article
- Steigerwald ML, Brus LE: Synthesis, stabilization and electronic structure of quantum semiconductor nanoclusters. Annu Rev Mater Sci 1989, 19: 471–495. 10.1146/annurev.ms.19.080189.002351View Article
- Sung Y–M, Park K-S, Lee Y–J, Kim T–G: Ripening kinetics of CdSe/ZnSe core/shell nanocrystals. J Phys Chem C 2007, 111: 1239–1242. 10.1021/jp066203cView Article
- Bilecka I, Elser P, Niederberger M: Kinetic and thermodynamic aspects in the microwave-assisted synthesis of ZnO nanoparticles in benzyl alcohol. ACS Nano 2009, 3: 467–477. 10.1021/nn800842bView Article
- Wei C-M, Hou S-S: Preparation and optical properties of blue-emitting colloidal CdS nanocrystallines by the solvothermal process using poly(ethylene oxide) as the stabilizer. Colloid Polym Sci 2007, 285: 1343–1349. 10.1007/s00396-007-1691-zView Article
- Bhattacharjee B, Ganguli D, Chaudhuri S: Growth behavior of CdS nanoparticles embedded in polymer and sol–gel silica matrices: relationship with surface-state-related luminescence. J Fluoresc 2002, 12: 369–375. 10.1023/A:1021305824793View Article
- Aşıkoğlu A, Yükselici MH: Evolution of the energy band structure in chemical bath deposited CdS thin films studied by optical absorption spectroscopy. Semicond Sci Technol 2011, 26: 1–5.
- Guglielmi M, Martucci A, Menegazzo E, Righini GC, Pelli S, Fick J, Vitrant G: Control of semiconductor particle size in sol–gel thin films. J Sol–Gel, Sci Technol 1997, 8: 1017–1021.
- Koç K, Tepehan FZ, Tepehan GG: Characterization of MPS capped CdS quantum dots and formation of self-assembled quantum dots thin films on a glassy substrate. Chalcogenide Lett 2011, 8: 239–247.
- Tong XL, Jiang DS, Liu ZM, Luo MZ, Li Y, Lu PX, Yang G, Long H: Structural characterization of CdS thin film on quartz formed by femtosecond pulsed laser deposition at high temperature. Thin Solid Films 2008, 516: 2003–2008. 10.1016/j.tsf.2007.06.067View Article
- Tremont R, Jesuâs-Cardona HD, Garcia-Orozco J, Castro RJ, Cabrera CR: 3-Mercaptopropyltrimethoxysilane as a Cu corrosion inhibitor in KCl solution. J Appl Electrochem 2000, 30: 737–743. 10.1023/A:1004072117517View Article
- Wuister SF, Meijerink A: Synthesis and luminescence of CdS quantum dots capped with a silica precursor. J Lumin 2003, 105: 35–43. 10.1016/S0022-2313(03)00095-4View Article
- Thielsch R, Böhme T, Böttcher H: Optical and structural properties of nanocrystalline ZnS-SiO2 composite films. Phys stat sol (a) 1996, 155: 157–170. 10.1002/pssa.2211550114View Article
- Rao CNR, Müller A: Nanomaterials chemistry. In Recent Developments and New Directions. Edited by: Cheetham AK. Weinheim: Wiley-Vch Verlag GmbH & Co; 2007.
- Zhang ZH, Chin WS, Vittal JJ: Water-soluble CdS quantum dots prepared from a refluxing single precursor in aqueous solution. J Phys Chem B 2004, 108: 18569–18574. 10.1021/jp0470849View Article
- Lam VQ, Turrell S, Martucci A, Bouazaoui M, Capoen B: Synthesis and optical properties of MPTMS-capped CdS quantum dots embedded in TiO2 thin films for photonic applications. J Non-Cryst Solids 2006, 352: 3315–3319. 10.1016/j.jnoncrysol.2006.02.096View Article
- Kundu M, Khosravi AA, Kulkarni SK: Synthesis and study of organically capped ultra small clusters of cadmium sulphide. J Mater Sci 1997, 32: 245–258. 10.1023/A:1018520425765View Article
- Brus LE: Electron–electron and electron–hole interactions in small semiconductor crystallites: the size dependence of the lowest excited electronic state. J Chem Phys 1984, 80: 4403–4409. 10.1063/1.447218View Article
- Kayanuma Y: Quantum-size effects of interacting electrons and holes in semiconductor microcrystals with spherical shape. Phys Rev B 1988, 38: 9797–9805. 10.1103/PhysRevB.38.9797View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.